# Elastic Properties of Materials ●

In document Fundamentals of Materials Science and Engineering 5th Edition pdf (Page 177-180)

where G is the shear modulus, the slope of the linear elastic region of the shear stress–strain curve. Table 7.1 also gives the shear moduli for a number of the common metals.

### 7.4 A

NELASTICITY

Up to this point, it has been assumed that elastic deformation is time independent, that is, that an applied stress produces an instantaneous elastic strain that remains constant over the period of time the stress is maintained. It has also been assumed that upon release of the load the strain is totally recovered, that is, that the strain immediately returns to zero. In most engineering materials, however, there will also exist a time-dependent elastic strain component. That is, elastic deformation will continue after the stress application, and upon load release some finite time is required for complete recovery. This time-dependent elastic behavior is known as

anelasticity, and it is due to time-dependent microscopic and atomistic processes

that are attendant to the deformation. For metals the anelastic component is nor- mally small and is often neglected. However, for some polymeric materials its magnitude is significant; in this case it is termedviscoelastic behavior,兵which is the discussion topic of Section 7.15.其

XAMPLE

ROBLEM

### 7.1

A piece of copper originally 305 mm (12 in.) long is pulled in tension with a stress of 276 MPa (40,000 psi). If the deformation is entirely elastic, what will be the resultant elongation?

### S

O L U T I O N

Since the deformation is elastic, strain is dependent on stress according to Equation 7.5. Furthermore, the elongation⌬l is related to the original length l0 through Equation 7.2. Combining these two expressions and solving for

l yields

␴⫽ ⑀E

l l0

### 冊

E

l⫽␴l0 E

The values of␴ and l0 are given as 276 MPa and 305 mm, respectively, and

the magnitude of E for copper from Table 7.1 is 110 GPa (16 ⫻ 106 psi).

Elongation is obtained by substitution into the expression above as

l⫽(276 MPa)(305 mm)

110⫻103MPa ⫽0.77 mm (0.03 in.)

LASTIC

ROPERTIES OF

### M

ATERIALS

When a tensile stress is imposed on virtually all materials, an elastic elongation and accompanying strain⑀zresult in the direction of the applied stress (arbitrarily

there will be constrictions in the lateral (x and y) directions perpendicular to the applied stress; from these contractions, the compressive strains ⑀x and ⑀y may be

determined. If the applied stress is uniaxial (only in the z direction), and the material is isotropic, then⑀x ⫽ ⑀y. A parameter termed Poisson’s ratio␯ is defined as the

ratio of the lateral and axial strains, or

␯⫽ ⫺ ⑀x

z

⫽ ⫺ ⑀y

z

(7.8)

The negative sign is included in the expression so that␯ will always be positive, since ⑀x and ⑀z will always be of opposite sign. Theoretically, Poisson’s ratio for

isotropic materials should be ; furthermore, the maximum value for ␯ (or that value for which there is no net volume change) is 0.50. For many metals and other alloys, values of Poisson’s ratio range between 0.25 and 0.35. Table 7.1 shows␯ values for several common materials; a more comprehensive list is given in Table B.3, Appendix B.

For isotropic materials, shear and elastic moduli are related to each other and to Poisson’s ratio according to

E2G(1⫹␯) (7.9)

In most metals G is about 0.4E; thus, if the value of one modulus is known, the other may be approximated.

Many materials are elastically anisotropic; that is, the elastic behavior (e.g., the magnitude of E) varies with crystallographic direction (see Table 3.7). For these materials the elastic properties are completely characterized only by the specification of several elastic constants, their number depending on characteristics of the crystal structure. Even for isotropic materials, for complete characterization of the elastic properties, at least two constants must be given. Since the grain orientation is random in most polycrystalline materials, these may be considered to be isotropic;

158Chapter 7 / Mechanical Properties

z y x l0z zz ␴ ⌬lz 2 ⌬lx 2 z ⑀ 2 ⌬lz/2 l0z = ⫺⑀x 2 ⌬lx/2 l0x = l0x

FIGURE7.9 Axial (z) elongation

(positive strain) and lateral (x and y) contractions (negative strains) in response to an imposed tensile stress. Solid lines represent dimensions after stress application; dashed lines, before.

7.5 Elastic Properties of Materials159

inorganic ceramic glasses are also isotropic. The remaining discussion of mechanical behavior assumes isotropy and polycrystallinity (for metals and crystalline ceramics) because such is the character of most engineering materials.

XAMPLE

ROBLEM

### 7.2

A tensile stress is to be applied along the long axis of a cylindrical brass rod that has a diameter of 10 mm (0.4 in.). Determine the magnitude of the load required to produce a 2.5 ⫻ 10⫺3 mm (10⫺4 in.) change in diameter if the

deformation is entirely elastic.

### S

O L U T I O N

This deformation situation is represented in the accompanying drawing.

When the force F is applied, the specimen will elongate in the z direction and at the same time experience a reduction in diameter,⌬d, of 2.5⫻10⫺3mm in

the x direction. For the strain in the x direction,

x⫽ ⌬ d d0 ⫽ ⫺ 2.5⫻10⫺3mm 10 mm ⫽ ⫺2.5⫻10 ⫺4

which is negative, since the diameter is reduced.

It next becomes necessary to calculate the strain in the z direction using Equation 7.8. The value for Poisson’s ratio for brass is 0.34 (Table 7.1), and thus

z⫽ ⫺ ⑀x

␯ ⫽ ⫺

(⫺2.5⫻10⫺4)

0.34 ⫽7.35⫻10

⫺4

The applied stress may now be computed using Equation 7.5 and the modulus of elasticity, given in Table 7.1 as 97 GPa (14⫻106psi), as

␴⫽ ⑀zE⫽(7.35⫻10⫺4)(97⫻ 103MPa)⫽71.3 MPa z F F x d0 di l0 lizll 0 li l0 l0 = ⑀xdd 0 di d0 d0 = = =

Finally, from Equation 7.1, the applied force may be determined as F⫽␴A0⫽␴

d0 2

### 冊

2 앟 ⫽(71.3⫻106N/m2)

10⫻10⫺ 3m 2

### 冊

2 앟⫽5600 N (1293 lbf)

### M E C H A N I C A L B E H A V I O R — M E T A L S

For most metallic materials, elastic deformation persists only to strains of about 0.005. As the material is deformed beyond this point, the stress is no longer proportional to strain (Hooke’s law, Equation 7.5, ceases to be valid), and permanent, nonrecoverable, or plastic deformation occurs. Figure 7.10a plots schematically the tensile stress–strain behavior into the plastic region for a typical metal. The transition from elastic to plastic is a gradual one for most metals; some curvature results at the onset of plastic deformation, which increases more rapidly with rising stress.

From an atomic perspective, plastic deformation corresponds to the breaking of bonds with original atom neighbors and then reforming bonds with new neighbors as large numbers of atoms or molecules move relative to one another; upon removal of the stress they do not return to their original positions. This permanent deforma- tion for metals is accomplished by means of a process called slip, which involves the motion of dislocations as discussed in Section 8.3.

ENSILE

### P

ROPERTIES

In document Fundamentals of Materials Science and Engineering 5th Edition pdf (Page 177-180)